ISSUES TO ADDRESS... • How does diffusion occur? • Why is it an important part of processing? • How can the rate of diffusion be predicted for some simple cases? • How does diffusion depend on structure and temperature? CHAPTER 6: DIFFUSION IN SOLIDS Gear from case-hardened steel (C diffusion)
Diffusion- Steady and Non-Steady State • Diffusion - Mass transport by atomic motion • Mechanisms • Gases & Liquids – random (Brownian) motion • Solids – vacancy diffusion or interstitial diffusion
Simple Diffusion • Glass tube filled with water. • At time t = 0, add some drops of ink to one end of the tube. • Measure the diffusion distance, x, over some time. • Compare the results with theory.
Inter-diffusion • Interdiffusion: In alloys, atoms tend to migrate from regions of large concentration. This is a diffusion couple. After some time Initially Adapted from Figs. 6.1 - 2, Callister 6e.
Self-diffusion • Self-diffusion: In an elemental solid, atoms also migrate. Label some atoms After some time
Substitution-diffusion:vacancies and interstitials • applies to substitutional impurities • atoms exchange with vacancies • rate depends on (1) number of vacancies; (2) activation energy to exchange. Number (or concentration*) of Vacancies at T • kBT gives eV * see web handout for derivation. E is an activation energy for a particular process (in J/mol, cal/mol, eV/atom).
increasing elapsed time Substitution-diffusion Vacancy Diffusion: • applies to substitutional impurities • atoms exchange with vacancies • rate depends on (1) number of vacancies; (2) activation energy to exchange.
Inter-diffusion across Interfaces • Rate of substitutional diffusion depends on: - vacancy concentration - frequency of jumping. (Courtesy P.M. Anderson) Why should interstitial diffusion be faster than by vacancy mode of diffusion?
Diffusion Mechanisms • Interstitial diffusion – smaller atoms diffuse between atoms. More rapid than vacancy diffusion
Processing using Diffusion • Case Hardening: -Diffuse carbon atoms into the host iron atoms at the surface. -Example of interstitial diffusion is a case hardened gear. Fig. 6.0, Callister 6e.(courtesy of Surface Div., Midland-Ross.) • Result: The "Case" is -hard to deform: C atoms "lock" planes from shearing. -hard to crack: C atoms put the surface in compression.
Processing using Diffusion • Doping Silicon with P for n-type semiconductors: • Process: 1. Deposit P rich layers on surface. Fig. 18.0, Callister 6e. 2. Heat it. 3. Result: Doped semiconductor regions.
Modeling rate of diffusion: flux diffused mass M Jslope time • Flux: • Directional Quantity • • Flux can be measured for: • - vacancies • - host (A) atoms • - impurity (B) atoms • Empirically determined: • – Make thin membrane of known surface area • – Impose concentration gradient • – Measure how fast atoms or molecules diffuse through the membrane A = Area of flow
Steady-state Diffusion: J ~ gradient of c • Concentration Profile, C(x): [kg/m3] Adapted from Fig. 6.2(c) • Fick's First Law: D is a constant! • The steeper the concentration profile, the greater the flux!
Steady-State Diffusion • Steady State:concentration profile not changing with time. • Apply Fick's First Law: • If Jx)left = Jx)right , then • Result: the slope, dC/dx, must be constant (i.e., slope doesn't vary with position)!
C1 C1 C2 x1 x2 C2 x Steady-State Diffusion Rate of diffusion independent of time • J ~ Fick’s first law of diffusion D diffusion coefficient
glove C1 paint remover skin C2 x1 x2 Example: Chemical Protection Clothing • Methylene chloride is a common ingredient of paint removers. Besides being an irritant, it also may be absorbed through skin. When using, protective gloves should be worn. • If butyl rubber gloves (0.04 cm thick) are used, what is the diffusive flux of methylene chloride through the glove? • Data: • D in butyl rubber: D = 110 x10-8 cm2/s • surface concentrations: • Diffusion distance: C1= 0.44 g/cm3 C2= 0.02 g/cm3 x2 – x1 = 0.04 cm
Example: C Diffusion in steel plate 700 C • Steel plate at 7000C with geometry shown: Adapted from Fig. 5.4, Callister 6e. Knowns: C1= 1.2 kg/m3 at 5mm (5 x 10–3 m) below surface. C2 = 0.8 kg/m3 at 10mm (1 x 10–2 m) below surface. D = 3 x10-11 m2/s at 700 C. • Q: In steady-state, how much carbon transfers from the rich to the deficient side?
Example: Diffusion of radioactive atoms • Surface of Ni plate at 10000C contains 50% Ni63 (radioactive) and 50% Ni (non-radioactive). • 4 microns below surface Ni63 /Ni = 48:52 • Lattice constant of Ni at 1000 C is 0.360 nm. • Experiment shows that self-diffusion of Ni is 1.6 x 10-9 cm2/sec What is the flux of Ni63 atoms through a plane 2 m below surface? How many Ni63 atoms/second through cell?
Where can we use Fick’s Law? • Fick's law is commonly used to model transport processes in • foods, • clothing, • biopolymers, • pharmaceuticals, • porous soils, • semiconductor doping process, etc. Example The total membrane surface area in the lungs (alveoli) may be on the order of 100 square meters and have a thickness of less than a millionth of a meter, so it is a very effective gas-exchange interface. CO2 in air has D~16 mm2/s, and, in water, D~ 0.0016 mm2/s
Non-Steady-State Diffusion • Concentration profile, C(x), changes w/ time. • To conserve matter: • Fick's First Law: • Governing Eqn.:
Non-Steady-State Diffusion: another look • Concentration profile, C(x), changes w/ time. • Rate of accumulation C(x) Fick’s 2nd Law • Using Fick’s Law: • If D is constant:
C s Non-Steady-State Diffusion: C = c(x,t) concentration of diffusing species is a function of both time and position • Copper diffuses into a bar of aluminum. B.C. at t = 0, C = Co for 0 x at t > 0, C = CS for x = 0 (fixed surface conc.) C = Co for x = Adapted from Fig. 6.5, Callister & Rethwisch 3e.
CS C(x,t) Co Non-Steady-State Diffusion • Cu diffuses into a bar of Al. • Solution: "error function” Values calibrated in Table 6.1
z erf(z) Using Table 6.1 find z where erf(z) = 0.8125. Use interpolation. 0.90 0.7970 z 0.8125 0.95 0.8209 z= 0.93 So, erf(z) = 0.8125 Now solve for D Example: Non-Steady-State Diffusion FCC iron-carbon alloy initially containing 0.20 wt% C is carburized at an elevated temperature and in an atmosphere that gives a surface C content at 1.0 wt%. If after49.5 h the concentration of carbon is 0.35 wt% at a position 4.0 mm below the surface, what temperature was treatment done? Solution
From Table 6.2, for diffusion of C in FCC Fe • Do = 2.3 x 10-5 m2/s Qd = 148,000 J/mol T = 1300 K = 1027°C Solution (cont.): • To solve for the temperature at which D has the above value, we use a rearranged form of Equation (6.9a); • D=D0 exp(-Qd/RT)
Example: Processing • Copper diffuses into a bar of aluminum. • 10 hours processed at 600 C gives desired C(x). • How many hours needed to get the same C(x) at 500 C? Key point 1: C(x,t500C) = C(x,t600C). Key point 2: Both cases have the same Co and Cs. • Result: Dt should be held constant. Note D(T) are T dependent! Values of D are provided. • Answer:
Diffusion Analysis • The experiment: we recorded combinations of t and x that kept C constant. = (constant here) • Diffusion depth given by:
Data from Diffusion Analysis • Experimental result: x ~ t0.58 • Theory predicts x ~ t0.50 from • Close agreement.
Diffusion and Temperature æ ö ç ÷ = D Do exp è ø Qd D = diffusion coefficient [m2/s] - Do R T = pre-exponential [m2/s] Qd = activation energy [J/mol or eV/atom] R = gas constant [8.314 J/mol-K] T = absolute temperature [K] • Diffusivity increases with T exponentially (so does Vacancy conc.). (see Table 6.2) Note:
Diffusion and Temperature T(C) 1500 1000 600 300 10-8 D (m2/s) C in g-Fe C in a-Fe 10-14 Fe in a-Fe Fe in g-Fe Al in Al 10-20 1000K/T 0.5 1.0 1.5 • Experimental Data: Adapted from Fig. 6.7, Adapted from Fig. 6.7, Callister & Rethwisch 3e. (Data for Fig. 6.7 from E.A. Brandes and G.B. Brook (Ed.) Smithells Metals Reference Book, 7th ed., Butterworth-Heinemann, Oxford, 1992.)
1000 1500 600 300 T(C) 10-8 D (m2/s) C in g-Fe C in a-Fe 10-14 Fe in a-Fe Fe in g-Fe Al in Al 10-20 1000K/T 0.5 1.0 1.5 Example: Comparing Diffuse in Fe Is C in fcc Fe diffusing faster than C in bcc Fe? • (Table 6.2) • fcc-Fe: D0=2.3x10–5(m2/2) • Q=1.53 eV/atom • T = 900 C D=5.9x10–12(m2/2) • bcc-Fe: D0=6.2x10–7(m2/2) • Q=0.83 eV/atom • T = 900 C D=1.7x10–10(m2/2) • • FCC Fe has both higher activation energy Q and D0 (holes larger in FCC). • BCC and FCC phase exist over limited range of T (at varying %C). • Hence, at same T, BCC diffuses faster due to lower Q. • Cannot always have the phase that you want at the %C and T you want! • which is why this is all important.
z-axis Connecting Holes, Diffusion, and Stress Red octahedral fcc Green + Red octahedral bcc FCC represented as a BCT cell, with relevant holes.
Other Types of Diffusion (Beside Atomic) • Flux is general concept: e.g. charges, phonons,… • Charge Flux – e = electric chg. N = net # e- cross A Defining conductivity (a material property) Solution: Fick’s 2nd Law Ohm’s Law • Heat Flux – • (by phonons) N = # of phonons with avg. energy Defining thermal conductivity (a material property) Solution: Fick’s 2nd Law Or w/ Thermal Diffusivity:
interface C1 C0 C2 Inter-diffusion (diffusion couples) Assuming DA = DB: C0 = (C1+C2)/2 Curve is symmetric about C0,
Cu Cu70Zn30 Cu t = 0 Zn concentration Mo wire markers After diffusion Kirkendall Effect: What if DA > DB? • Kirkendall studied Mo markers in Cu-brass (i.e., fcc Cu70Zn30). • Symmetry is lost: Zn atoms move more readily in one direction (to the right) than Cu atoms move in the other (to the left). • When diffusion is asymmetric, interface moves away markers, • i.e., there is a net flow of atoms to the right past the markers. • Analyzing movement of markers determines DZn and DCu. • Kirkendall effect driven by vacancies, effective for T > 0.5 Tmelt.
O Ni O Ni O Ni O Ni O O Ni2+ O2– Ni Ni O Ni2+ O2– Ni O2– + O Ni – Ni2+ O Ni O Ni O Ni O Ni O Ni O Diffusion in Compounds: Ionic Conductors • Unlike diffusion in metals, diffusion in compounds involves second-neighbor migration. • Since the activation energies are high, the D’s are low unless vacancies are present from non-stoichiometric ratios of atoms. e.g., NiO There are Schottky defects • The two vacancies cannot accept neighbors because they have wrong charge, and ion diffusion needs 2nd neighbors with high barriers (activation energies).
Diffusion in Compounds: Ionic Conductors • D’s in an ionic compound are seldom comparable because of size, change and/or structural differences. • Two sources of conduction: ion diffusion and via e- hopping from ions of variable valency, e.g., Fe2+ to Fe3+, in applied electric field. • e.g., ionic • In NaCl at 1000 K, DNa+~ 5DCl– ,whereas at 825 K DNa+ ~ 50DCl–! • This is primarily due to size rNa+ = 1 A vs rCl–=1.8 A. • e.g., oxides • In uranium oxide, U4+(O2–)2, at 1000 K (extrapolated), DO ~ 107 DU. • This is mostly due to charge, i.e. more energy to activate 4+ U ion. • Also, UO is not stoichiometric, having U3+ ions to give UO2-x, so that the anion vacancies significantly increase O2- mobility. • e.g., solid-solutions of oxides (leads to defects, e.g., vacancies) • If Fe1-xO (x=2.5-4% at 1500 K, 3Fe2+ -> 2Fe3+ + vac.) is dissolved in MgO under reducing conditions, then Mg2+ diffusion increases. • If MgF2is dissolved in LiF (2Li+ -> Mg2+ + vac.), then Li+ diffusion increases. All due to additional vacancies.
Ionic Conduction: related to fuel cells • Molten salts and aqueous electrolytes conduct charge when placed in electric field, +q and –q move in opposite directions. • The same occurs in solids although at much slower rate. • Each ion has charge of Ze(e = 1.6 x 10–19 amp*sec), • so ion movement induces ionic conduction • Conductivity is related to mobility, , which is related to D via the Einstein equations: • Hence So, electrical conduction can be used determine diffusion data in ionic solids. • e.g., What conductivity results by Ca2+ diffusion in CaO at 2000 K? • CaO has NaCl structure with a= 4.81 A, with D(2000 K)~10-14m2/s, and Z=2.
Example: solid-oxide fuel cell (SOFC) • SOFC is made up of four layers, three of which are ceramics (hence the name). • A single cell consisting of these four layers stacked together is only a few mm thick. • Need to stack many, many together to have larger DC current. Overall: H2+ 1/2O2 H2O H2 2H++2e– O2–+ 2H+ + 2e– H2O Image: http://www.ip3.unipg.it/FuelCells/en/htfc.asp S. Haile’s SOFC (2004 best): Thin-film of Sm-doped Ceria electrolyte (CeO2, i.e. SmxCe1-xO2-x/2) and BSCF cathode (Perovskite Ba0.5Sr0.5Co0.8Fe0.2O3-d) show high power densities – over 1 W/cm2 at 600 C – with humidified H2 as the fuel and air at the cathode.
Holes for diffusion Ceramic Compounds: Al2O3 Unit cell defined by Al ions: 2 Al + 3 O
Summary: Structure and Diffusion Diffusion FASTER for... • open crystal structures • lower melting T materials • materials w/secondary bonding • smaller diffusing atoms • cations • lower density materials Diffusion SLOWER for... • close-packed structures • higher melting T materials • materials w/covalent bonding • larger diffusing atoms • anions • higher density materials